 
data_1 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'Li O4 P Rb2' 
_chemical_formula_weight          272.85 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'Li'  'Li'  -0.0003   0.0001 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'P'  'P'   0.1023   0.0942 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Rb'  'Rb'  -0.9393   2.9676 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            'Orthorhombic'
_symmetry_space_group_name_H-M    'Cmc2(1)' 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, z+1/2' 
 'x, -y, z+1/2' 
 '-x, y, z' 
 'x+1/2, y+1/2, z' 
 '-x+1/2, -y+1/2, z+1/2' 
 'x+1/2, -y+1/2, z+1/2' 
 '-x+1/2, y+1/2, z' 
 
_cell_length_a                    5.624(7) 
_cell_length_b                    11.351(14) 
_cell_length_c                    7.744(9) 
_cell_angle_alpha                 90.00 
_cell_angle_beta                  90.00 
_cell_angle_gamma                 90.00 
_cell_volume                      494.3(10) 
_cell_formula_units_Z             4 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     1092 
_cell_measurement_theta_min       3.59 
_cell_measurement_theta_max       27.58
 
_exptl_crystal_description        block
_exptl_crystal_colour             colorless
_exptl_crystal_size_max           0.245 
_exptl_crystal_size_mid           0.17 
_exptl_crystal_size_min           0.168
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.666 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              496 
_exptl_absorpt_coefficient_mu     20.020 
_exptl_absorpt_correction_type    'numerical'
_exptl_absorpt_correction_T_min   0.3184  
_exptl_absorpt_correction_T_max   1.0000 
_exptl_absorpt_process_details    "Face-indexed"  
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'CCD area detector'
_diffrn_measurement_method        'phi and omega scans' 
_diffrn_detector_area_resol_mean  ? 
_diffrn_standards_number          ? 
_diffrn_standards_interval_count  ? 
_diffrn_standards_interval_time   ? 
_diffrn_standards_decay_%         ? 
_diffrn_reflns_number             1432 
_diffrn_reflns_av_R_equivalents   0.0468 
_diffrn_reflns_av_sigmaI/netI     0.0671 
_diffrn_reflns_limit_h_min        -7 
_diffrn_reflns_limit_h_max        5 
_diffrn_reflns_limit_k_min        -13 
_diffrn_reflns_limit_k_max        14 
_diffrn_reflns_limit_l_min        -10 
_diffrn_reflns_limit_l_max        10 
_diffrn_reflns_theta_min          3.59 
_diffrn_reflns_theta_max          27.59 
_reflns_number_total              623 
_reflns_number_gt                 599 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        'Bruker SMART' 
_computing_cell_refinement        'Bruker SMART'
_computing_data_reduction         'Bruker SAINT' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL'
_computing_publication_material   'Bruker SHELXTL'
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0049P)²+0.0000P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    ? 
_refine_ls_hydrogen_treatment     ? 
_refine_ls_extinction_method      SHELXL 
_refine_ls_extinction_coef        0.0159(13) 
_refine_ls_extinction_expression 
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^' 
_refine_ls_abs_structure_details 
 'Flack H D (1983), Acta Cryst. A39, 876-881' 
_refine_ls_abs_structure_Flack    0.032(19) 
_refine_ls_number_reflns          623 
_refine_ls_number_parameters      44 
_refine_ls_number_restraints      1 
_refine_ls_R_factor_all           0.0323 
_refine_ls_R_factor_gt            0.0304 
_refine_ls_wR_factor_ref          0.0679 
_refine_ls_wR_factor_gt           0.0675 
_refine_ls_goodness_of_fit_ref    1.033 
_refine_ls_restrained_S_all       1.032 
_refine_ls_shift/su_max           0.000 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Li1 Li 0.5000 0.2056(14) 0.0274(18) 0.012(3) Uiso 1 2 d S . . 
Rb1 Rb 0.0000 0.10610(7) -0.20742(9) 0.0149(3) Uani 1 2 d S . . 
Rb2 Rb 0.0000 0.43594(7) -0.05767(11) 0.0157(3) Uani 1 2 d S . . 
P1 P 0.0000 0.1931(2) 0.2391(2) 0.0078(4) Uani 1 2 d S . . 
O1 O 0.0000 0.1344(5) 0.4197(8) 0.0116(12) Uani 1 2 d S . . 
O2 O 0.0000 0.3281(5) 0.2711(7) 0.0145(13) Uani 1 2 d S . . 
O3 O 0.2232(8) 0.1567(4) 0.1394(6) 0.0175(9) Uani 1 1 d . . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Li1 O3 1.866(10) . ? 
Li1 O3 1.866(10) 4_655 ? 
Li1 O1 1.999(17) 6_554 ? 
Li1 O2 2.021(16) 6_554 ? 
Li1 P1 2.511(15) 6_554 ? 
Li1 Rb1 2.964(15) 6 ? 
Li1 Rb2 3.131(16) 5_545 ? 
Li1 Rb1 3.534(9) . ? 
Li1 Rb1 3.534(9) 1_655 ? 
Li1 Rb2 3.592(15) 6 ? 
Li1 Rb2 3.896(11) 1_655 ? 
Li1 Rb2 3.896(11) . ? 
Rb1 O1 2.902(6) 2_554 ? 
Rb1 O1 2.906(7) 1_554 ? 
Rb1 O2 2.914(4) 6_554 ? 
Rb1 O2 2.914(4) 6_454 ? 
Rb1 Li1 2.964(15) 6_554 ? 
Rb1 O3 3.020(6) . ? 
Rb1 O3 3.020(6) 4 ? 
Rb1 O3 3.328(5) 6_554 ? 
Rb1 O3 3.328(5) 7_454 ? 
Rb1 P1 3.421(5) 2_554 ? 
Rb1 O3 3.447(6) 2_554 ? 
Rb1 O3 3.447(6) 3_554 ? 
Rb2 O2 2.825(6) . ? 
Rb2 O1 2.928(4) 6_454 ? 
Rb2 O1 2.928(4) 6_554 ? 
Rb2 O2 2.988(6) 2_564 ? 
Rb2 O3 3.005(5) 7_454 ? 
Rb2 O3 3.005(5) 6_554 ? 
Rb2 Li1 3.131(16) 5_455 ? 
Rb2 O3 3.322(5) 8 ? 
Rb2 O3 3.322(5) 5_455 ? 
Rb2 P1 3.539(3) 6_454 ? 
Rb2 P1 3.539(3) 6_554 ? 
Rb2 P1 3.589(4) . ? 
P1 O3 1.530(5) 4 ? 
P1 O3 1.530(5) . ? 
P1 O1 1.548(6) . ? 
P1 O2 1.553(6) . ? 
P1 Li1 2.511(15) 6 ? 
P1 Rb1 3.421(5) 2 ? 
P1 Rb2 3.539(3) 6 ? 
P1 Rb2 3.539(3) 6_455 ? 
P1 Rb1 3.644(3) 6 ? 
P1 Rb1 3.644(3) 6_455 ? 
O1 Li1 1.999(17) 6 ? 
O1 Rb1 2.902(6) 2 ? 
O1 Rb1 2.906(7) 1_556 ? 
O1 Rb2 2.928(4) 6_455 ? 
O1 Rb2 2.928(4) 6 ? 
O2 Li1 2.021(16) 6 ? 
O2 Rb1 2.914(4) 6 ? 
O2 Rb1 2.914(4) 6_455 ? 
O2 Rb2 2.988(6) 2_565 ? 
O3 Rb2 3.005(5) 6 ? 
O3 Rb2 3.322(5) 5_545 ? 
O3 Rb1 3.328(5) 6 ? 
O3 Rb1 3.447(6) 2 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O3 Li1 O3 113.0(8) . 4_655 ? 
O3 Li1 O1 117.7(5) . 6_554 ? 
O3 Li1 O1 117.7(5) 4_655 6_554 ? 
O3 Li1 O2 113.6(5) . 6_554 ? 
O3 Li1 O2 113.6(5) 4_655 6_554 ? 
O1 Li1 O2 76.3(5) 6_554 6_554 ? 
O3 Li1 P1 123.3(4) . 6_554 ? 
O3 Li1 P1 123.3(4) 4_655 6_554 ? 
O1 Li1 P1 38.1(3) 6_554 6_554 ? 
O2 Li1 P1 38.2(3) 6_554 6_554 ? 
O3 Li1 Rb1 83.8(5) . 6 ? 
O3 Li1 Rb1 83.8(5) 4_655 6 ? 
O1 Li1 Rb1 68.5(5) 6_554 6 ? 
O2 Li1 Rb1 144.8(7) 6_554 6 ? 
P1 Li1 Rb1 106.6(5) 6_554 6 ? 
O3 Li1 Rb2 78.9(5) . 5_545 ? 
O3 Li1 Rb2 78.9(5) 4_655 5_545 ? 
O1 Li1 Rb2 143.2(6) 6_554 5_545 ? 
O2 Li1 Rb2 66.9(4) 6_554 5_545 ? 
P1 Li1 Rb2 105.1(5) 6_554 5_545 ? 
Rb1 Li1 Rb2 148.3(5) 6 5_545 ? 
O3 Li1 Rb1 58.7(3) . . ? 
O3 Li1 Rb1 143.9(7) 4_655 . ? 
O1 Li1 Rb1 94.3(4) 6_554 . ? 
O2 Li1 Rb1 55.5(2) 6_554 . ? 
P1 Li1 Rb1 71.9(3) 6_554 . ? 
Rb1 Li1 Rb1 125.9(2) 6 . ? 
Rb2 Li1 Rb1 65.1(2) 5_545 . ? 
O3 Li1 Rb1 143.9(7) . 1_655 ? 
O3 Li1 Rb1 58.7(3) 4_655 1_655 ? 
O1 Li1 Rb1 94.3(4) 6_554 1_655 ? 
O2 Li1 Rb1 55.5(2) 6_554 1_655 ? 
P1 Li1 Rb1 71.9(3) 6_554 1_655 ? 
Rb1 Li1 Rb1 125.9(2) 6 1_655 ? 
Rb2 Li1 Rb1 65.1(2) 5_545 1_655 ? 
Rb1 Li1 Rb1 105.4(4) . 1_655 ? 
O3 Li1 Rb2 56.7(4) . 6 ? 
O3 Li1 Rb2 56.7(4) 4_655 6 ? 
O1 Li1 Rb2 141.2(6) 6_554 6 ? 
O2 Li1 Rb2 142.5(7) 6_554 6 ? 
P1 Li1 Rb2 179.3(6) 6_554 6 ? 
Rb1 Li1 Rb2 72.7(3) 6 6 ? 
Rb2 Li1 Rb2 75.6(3) 5_545 6 ? 
Rb1 Li1 Rb2 108.5(3) . 6 ? 
Rb1 Li1 Rb2 108.5(3) 1_655 6 ? 
O3 Li1 Rb2 151.7(7) . 1_655 ? 
O3 Li1 Rb2 71.1(3) 4_655 1_655 ? 
O1 Li1 Rb2 47.12(18) 6_554 1_655 ? 
O2 Li1 Rb2 87.8(4) 6_554 1_655 ? 
P1 Li1 Rb2 62.8(2) 6_554 1_655 ? 
Rb1 Li1 Rb2 68.5(3) 6 1_655 ? 
Rb2 Li1 Rb2 128.4(2) 5_545 1_655 ? 
Rb1 Li1 Rb2 134.6(4) . 1_655 ? 
Rb1 Li1 Rb2 63.46(13) 1_655 1_655 ? 
Rb2 Li1 Rb2 116.8(3) 6 1_655 ? 
O3 Li1 Rb2 71.1(3) . . ? 
O3 Li1 Rb2 151.7(7) 4_655 . ? 
O1 Li1 Rb2 47.12(18) 6_554 . ? 
O2 Li1 Rb2 87.8(4) 6_554 . ? 
P1 Li1 Rb2 62.8(3) 6_554 . ? 
Rb1 Li1 Rb2 68.5(3) 6 . ? 
Rb2 Li1 Rb2 128.4(2) 5_545 . ? 
Rb1 Li1 Rb2 63.46(13) . . ? 
Rb1 Li1 Rb2 134.6(4) 1_655 . ? 
Rb2 Li1 Rb2 116.8(3) 6 . ? 
Rb2 Li1 Rb2 92.4(3) 1_655 . ? 
O1 Rb1 O1 116.17(14) 2_554 1_554 ? 
O1 Rb1 O2 105.09(10) 2_554 6_554 ? 
O1 Rb1 O2 85.13(11) 1_554 6_554 ? 
O1 Rb1 O2 105.09(10) 2_554 6_454 ? 
O1 Rb1 O2 85.13(11) 1_554 6_454 ? 
O2 Rb1 O2 149.6(2) 6_554 6_454 ? 
O1 Rb1 Li1 156.0(3) 2_554 6_554 ? 
O1 Rb1 Li1 39.8(3) 1_554 6_554 ? 
O2 Rb1 Li1 77.04(11) 6_554 6_554 ? 
O2 Rb1 Li1 77.04(11) 6_454 6_554 ? 
O1 Rb1 O3 82.96(15) 2_554 . ? 
O1 Rb1 O3 149.65(11) 1_554 . ? 
O2 Rb1 O3 66.48(14) 6_554 . ? 
O2 Rb1 O3 113.77(14) 6_454 . ? 
Li1 Rb1 O3 118.6(3) 6_554 . ? 
O1 Rb1 O3 82.96(15) 2_554 4 ? 
O1 Rb1 O3 149.65(11) 1_554 4 ? 
O2 Rb1 O3 113.77(14) 6_554 4 ? 
O2 Rb1 O3 66.48(14) 6_454 4 ? 
Li1 Rb1 O3 118.6(3) 6_554 4 ? 
O3 Rb1 O3 49.12(18) . 4 ? 
O1 Rb1 O3 151.86(9) 2_554 6_554 ? 
O1 Rb1 O3 63.67(13) 1_554 6_554 ? 
O2 Rb1 O3 47.25(13) 6_554 6_554 ? 
O2 Rb1 O3 102.93(14) 6_454 6_554 ? 
Li1 Rb1 O3 33.88(18) 6_554 6_554 ? 
O3 Rb1 O3 88.20(9) . 6_554 ? 
O3 Rb1 O3 110.94(9) 4 6_554 ? 
O1 Rb1 O3 151.86(9) 2_554 7_454 ? 
O1 Rb1 O3 63.67(13) 1_554 7_454 ? 
O2 Rb1 O3 102.93(14) 6_554 7_454 ? 
O2 Rb1 O3 47.25(13) 6_454 7_454 ? 
Li1 Rb1 O3 33.88(18) 6_554 7_454 ? 
O3 Rb1 O3 110.94(9) . 7_454 ? 
O3 Rb1 O3 88.20(9) 4 7_454 ? 
O3 Rb1 O3 55.77(17) 6_554 7_454 ? 
O1 Rb1 P1 26.77(13) 2_554 2_554 ? 
O1 Rb1 P1 89.40(12) 1_554 2_554 ? 
O2 Rb1 P1 104.32(11) 6_554 2_554 ? 
O2 Rb1 P1 104.32(11) 6_454 2_554 ? 
Li1 Rb1 P1 129.2(3) 6_554 2_554 ? 
O3 Rb1 P1 107.24(10) . 2_554 ? 
O3 Rb1 P1 107.24(10) 4 2_554 ? 
O3 Rb1 P1 139.45(10) 6_554 2_554 ? 
O3 Rb1 P1 139.45(10) 7_454 2_554 ? 
O1 Rb1 O3 45.77(14) 2_554 2_554 ? 
O1 Rb1 O3 75.74(14) 1_554 2_554 ? 
O2 Rb1 O3 123.61(13) 6_554 2_554 ? 
O2 Rb1 O3 81.41(14) 6_454 2_554 ? 
Li1 Rb1 O3 112.7(3) 6_554 2_554 ? 
O3 Rb1 O3 128.46(11) . 2_554 ? 
O3 Rb1 O3 108.62(13) 4 2_554 ? 
O3 Rb1 O3 138.40(16) 6_554 2_554 ? 
O3 Rb1 O3 114.02(12) 7_454 2_554 ? 
P1 Rb1 O3 25.75(8) 2_554 2_554 ? 
O1 Rb1 O3 45.77(14) 2_554 3_554 ? 
O1 Rb1 O3 75.74(14) 1_554 3_554 ? 
O2 Rb1 O3 81.41(14) 6_554 3_554 ? 
O2 Rb1 O3 123.61(13) 6_454 3_554 ? 
Li1 Rb1 O3 112.7(3) 6_554 3_554 ? 
O3 Rb1 O3 108.62(13) . 3_554 ? 
O3 Rb1 O3 128.46(11) 4 3_554 ? 
O3 Rb1 O3 114.02(12) 6_554 3_554 ? 
O3 Rb1 O3 138.40(16) 7_454 3_554 ? 
P1 Rb1 O3 25.75(8) 2_554 3_554 ? 
O3 Rb1 O3 42.71(16) 2_554 3_554 ? 
O2 Rb2 O1 86.33(12) . 6_454 ? 
O2 Rb2 O1 86.33(12) . 6_554 ? 
O1 Rb2 O1 147.6(2) 6_454 6_554 ? 
O2 Rb2 O2 142.01(15) . 2_564 ? 
O1 Rb2 O2 102.57(11) 6_454 2_564 ? 
O1 Rb2 O2 102.57(11) 6_554 2_564 ? 
O2 Rb2 O3 123.50(14) . 7_454 ? 
O1 Rb2 O3 50.24(15) 6_454 7_454 ? 
O1 Rb2 O3 110.81(14) 6_554 7_454 ? 
O2 Rb2 O3 88.13(14) 2_564 7_454 ? 
O2 Rb2 O3 123.50(14) . 6_554 ? 
O1 Rb2 O3 110.81(14) 6_454 6_554 ? 
O1 Rb2 O3 50.24(15) 6_554 6_554 ? 
O2 Rb2 O3 88.13(14) 2_564 6_554 ? 
O3 Rb2 O3 62.40(19) 7_454 6_554 ? 
O2 Rb2 Li1 103.5(3) . 5_455 ? 
O1 Rb2 Li1 106.21(11) 6_454 5_455 ? 
O1 Rb2 Li1 106.21(11) 6_554 5_455 ? 
O2 Rb2 Li1 38.5(3) 2_564 5_455 ? 
O3 Rb2 Li1 120.4(2) 7_454 5_455 ? 
O3 Rb2 Li1 120.4(2) 6_554 5_455 ? 
O2 Rb2 O3 84.99(15) . 8 ? 
O1 Rb2 O3 133.10(14) 6_454 8 ? 
O1 Rb2 O3 77.48(14) 6_554 8 ? 
O2 Rb2 O3 61.82(14) 2_564 8 ? 
O3 Rb2 O3 149.94(11) 7_454 8 ? 
O3 Rb2 O3 112.33(15) 6_554 8 ? 
Li1 Rb2 O3 33.46(16) 5_455 8 ? 
O2 Rb2 O3 84.99(15) . 5_455 ? 
O1 Rb2 O3 77.48(15) 6_454 5_455 ? 
O1 Rb2 O3 133.10(14) 6_554 5_455 ? 
O2 Rb2 O3 61.82(14) 2_564 5_455 ? 
O3 Rb2 O3 112.33(15) 7_454 5_455 ? 
O3 Rb2 O3 149.94(11) 6_554 5_455 ? 
Li1 Rb2 O3 33.46(17) 5_455 5_455 ? 
O3 Rb2 O3 55.90(17) 8 5_455 ? 
O2 Rb2 P1 102.79(9) . 6_454 ? 
O1 Rb2 P1 25.53(12) 6_454 6_454 ? 
O1 Rb2 P1 128.57(13) 6_554 6_454 ? 
O2 Rb2 P1 99.99(9) 2_564 6_454 ? 
O3 Rb2 P1 25.40(9) 7_454 6_454 ? 
O3 Rb2 P1 85.40(12) 6_554 6_454 ? 
Li1 Rb2 P1 119.87(11) 5_455 6_454 ? 
O3 Rb2 P1 152.72(9) 8 6_454 ? 
O3 Rb2 P1 98.28(11) 5_455 6_454 ? 
O2 Rb2 P1 102.79(9) . 6_554 ? 
O1 Rb2 P1 128.57(13) 6_454 6_554 ? 
O1 Rb2 P1 25.53(12) 6_554 6_554 ? 
O2 Rb2 P1 99.99(9) 2_564 6_554 ? 
O3 Rb2 P1 85.40(12) 7_454 6_554 ? 
O3 Rb2 P1 25.40(9) 6_554 6_554 ? 
Li1 Rb2 P1 119.87(11) 5_455 6_554 ? 
O3 Rb2 P1 98.28(11) 8 6_554 ? 
O3 Rb2 P1 152.72(9) 5_455 6_554 ? 
P1 Rb2 P1 105.22(10) 6_454 6_554 ? 
O2 Rb2 P1 24.51(11) . . ? 
O1 Rb2 P1 80.15(11) 6_454 . ? 
O1 Rb2 P1 80.15(11) 6_554 . ? 
O2 Rb2 P1 166.52(12) 2_564 . ? 
O3 Rb2 P1 103.36(12) 7_454 . ? 
O3 Rb2 P1 103.36(12) 6_554 . ? 
Li1 Rb2 P1 128.0(3) 5_455 . ? 
O3 Rb2 P1 106.57(12) 8 . ? 
O3 Rb2 P1 106.57(12) 5_455 . ? 
P1 Rb2 P1 88.10(6) 6_454 . ? 
P1 Rb2 P1 88.10(6) 6_554 . ? 
O3 P1 O3 110.2(4) 4 . ? 
O3 P1 O1 109.8(2) 4 . ? 
O3 P1 O1 109.8(2) . . ? 
O3 P1 O2 110.3(2) 4 . ? 
O3 P1 O2 110.3(2) . . ? 
O1 P1 O2 106.3(3) . . ? 
O3 P1 Li1 124.89(19) 4 6 ? 
O3 P1 Li1 124.89(19) . 6 ? 
O1 P1 Li1 52.7(4) . 6 ? 
O2 P1 Li1 53.6(4) . 6 ? 
O3 P1 Rb1 78.1(2) 4 2 ? 
O3 P1 Rb1 78.1(2) . 2 ? 
O1 P1 Rb1 57.6(2) . 2 ? 
O2 P1 Rb1 163.9(2) . 2 ? 
Li1 P1 Rb1 110.3(4) 6 2 ? 
O3 P1 Rb2 139.9(2) 4 6 ? 
O3 P1 Rb2 57.4(2) . 6 ? 
O1 P1 Rb2 54.60(7) . 6 ? 
O2 P1 Rb2 109.73(13) . 6 ? 
Li1 P1 Rb2 78.1(2) 6 6 ? 
Rb1 P1 Rb2 62.32(5) 2 6 ? 
O3 P1 Rb2 57.4(2) 4 6_455 ? 
O3 P1 Rb2 139.9(2) . 6_455 ? 
O1 P1 Rb2 54.60(7) . 6_455 ? 
O2 P1 Rb2 109.73(13) . 6_455 ? 
Li1 P1 Rb2 78.1(2) 6 6_455 ? 
Rb1 P1 Rb2 62.32(5) 2 6_455 ? 
Rb2 P1 Rb2 105.22(10) 6 6_455 ? 
O3 P1 Rb2 83.3(2) 4 . ? 
O3 P1 Rb2 83.3(2) . . ? 
O1 P1 Rb2 155.3(2) . . ? 
O2 P1 Rb2 49.0(2) . . ? 
Li1 P1 Rb2 102.6(4) 6 . ? 
Rb1 P1 Rb2 147.13(7) 2 . ? 
Rb2 P1 Rb2 127.04(5) 6 . ? 
Rb2 P1 Rb2 127.04(5) 6_455 . ? 
O3 P1 Rb1 56.00(19) 4 . ? 
O3 P1 Rb1 56.00(19) . . ? 
O1 P1 Rb1 138.6(2) . . ? 
O2 P1 Rb1 115.1(2) . . ? 
Li1 P1 Rb1 168.7(4) 6 . ? 
Rb1 P1 Rb1 81.01(6) 2 . ? 
Rb2 P1 Rb1 108.29(6) 6 . ? 
Rb2 P1 Rb1 108.29(6) 6_455 . ? 
Rb2 P1 Rb1 66.11(8) . . ? 
O3 P1 Rb1 149.2(2) 4 6 ? 
O3 P1 Rb1 65.98(19) . 6 ? 
O1 P1 Rb1 99.59(15) . 6 ? 
O2 P1 Rb1 50.52(5) . 6 ? 
Li1 P1 Rb1 67.2(2) 6 6 ? 
Rb1 P1 Rb1 127.40(6) 2 6 ? 
Rb2 P1 Rb1 66.12(8) 6 6 ? 
Rb2 P1 Rb1 145.24(7) 6_455 6 ? 
Rb2 P1 Rb1 65.93(6) . 6 ? 
Rb1 P1 Rb1 106.32(5) . 6 ? 
O3 P1 Rb1 65.98(19) 4 6_455 ? 
O3 P1 Rb1 149.2(2) . 6_455 ? 
O1 P1 Rb1 99.59(15) . 6_455 ? 
O2 P1 Rb1 50.52(5) . 6_455 ? 
Li1 P1 Rb1 67.2(2) 6 6_455 ? 
Rb1 P1 Rb1 127.40(6) 2 6_455 ? 
Rb2 P1 Rb1 145.24(8) 6 6_455 ? 
Rb2 P1 Rb1 66.12(8) 6_455 6_455 ? 
Rb2 P1 Rb1 65.93(6) . 6_455 ? 
Rb1 P1 Rb1 106.32(5) . 6_455 ? 
Rb1 P1 Rb1 101.03(11) 6 6_455 ? 
P1 O1 Li1 89.2(5) . 6 ? 
P1 O1 Rb1 95.7(3) . 2 ? 
Li1 O1 Rb1 175.2(5) 6 2 ? 
P1 O1 Rb1 160.9(3) . 1_556 ? 
Li1 O1 Rb1 71.7(4) 6 1_556 ? 
Rb1 O1 Rb1 103.48(19) 2 1_556 ? 
P1 O1 Rb2 99.87(13) . 6_455 ? 
Li1 O1 Rb2 102.87(13) 6 6_455 ? 
Rb1 O1 Rb2 76.34(11) 2 6_455 ? 
Rb1 O1 Rb2 84.85(12) 1_556 6_455 ? 
P1 O1 Rb2 99.87(13) . 6 ? 
Li1 O1 Rb2 102.87(13) 6 6 ? 
Rb1 O1 Rb2 76.34(11) 2 6 ? 
Rb1 O1 Rb2 84.85(12) 1_556 6 ? 
Rb2 O1 Rb2 147.6(2) 6_455 6 ? 
P1 O2 Li1 88.3(5) . 6 ? 
P1 O2 Rb2 106.5(3) . . ? 
Li1 O2 Rb2 165.3(5) 6 . ? 
P1 O2 Rb1 105.19(10) . 6 ? 
Li1 O2 Rb1 89.57(16) 6 6 ? 
Rb2 O2 Rb1 86.59(11) . 6 ? 
P1 O2 Rb1 105.19(10) . 6_455 ? 
Li1 O2 Rb1 89.57(16) 6 6_455 ? 
Rb2 O2 Rb1 86.59(11) . 6_455 ? 
Rb1 O2 Rb1 149.6(2) 6 6_455 ? 
P1 O2 Rb2 162.8(3) . 2_565 ? 
Li1 O2 Rb2 74.6(5) 6 2_565 ? 
Rb2 O2 Rb2 90.67(17) . 2_565 ? 
Rb1 O2 Rb2 75.24(10) 6 2_565 ? 
Rb1 O2 Rb2 75.24(10) 6_455 2_565 ? 
P1 O3 Li1 147.0(6) . . ? 
P1 O3 Rb2 97.2(2) . 6 ? 
Li1 O3 Rb2 92.0(4) . 6 ? 
P1 O3 Rb1 99.2(2) . . ? 
Li1 O3 Rb1 89.4(4) . . ? 
Rb2 O3 Rb1 147.45(17) 6 . ? 
P1 O3 Rb2 145.1(3) . 5_545 ? 
Li1 O3 Rb2 67.7(5) . 5_545 ? 
Rb2 O3 Rb2 81.48(13) 6 5_545 ? 
Rb1 O3 Rb2 69.06(11) . 5_545 ? 
P1 O3 Rb1 89.2(2) . 6 ? 
Li1 O3 Rb1 62.3(5) . 6 ? 
Rb2 O3 Rb1 76.27(12) 6 6 ? 
Rb1 O3 Rb1 131.70(16) . 6 ? 
Rb2 O3 Rb1 123.70(15) 5_545 6 ? 
P1 O3 Rb1 76.2(2) . 2 ? 
Li1 O3 Rb1 136.1(5) . 2 ? 
Rb2 O3 Rb1 67.50(11) 6 2 ? 
Rb1 O3 Rb1 89.42(13) . 2 ? 
Rb2 O3 Rb1 71.08(12) 5_545 2 ? 
Rb1 O3 Rb1 138.40(16) 6 2 ? 
 
_diffrn_measured_fraction_theta_max    1.000 
_diffrn_reflns_theta_full              27.59 
_diffrn_measured_fraction_theta_full   1.000 
_refine_diff_density_max    1.237 
_refine_diff_density_min   -1.023 
_refine_diff_density_rms    0.209 
